# Effect of Fullerene Derivates on Thermal and Crystallization Behavior of PBT/Decylamine-C60 and PBT/TCNEO-C60 Nanocomposites

Authors: A. Woźniak-Braszak; K. Jurga; J. Jurga; M. Baranowski; W. Grzesiak; B. Brycki; K. Hołderna-Natkaniec
Journal: Journal of Nanomaterials
 (2012)

---

## Abstract

The paper describes the process of the preparation of new nanocomposites based on poly(butylene terephthalate) and C60 nanoparticles modified by decylamine (DA) and tetracyanoethylene oxide (TCNEO), respectively. Thermal and crystallization properties of new synthesized nanocomposites were investigated by means of thermal differential scanning calorimetry (DSC). The experimental results demonstrate the effect of fullerene derivates, DA-C60 and TCNEO-C60, on the melting and crystallinity processes of nanocomposites. The morphology of new nanocomposites was investigated by SEM.


---

## Body

## 1. Introduction

Recently, nanocomposites have received great attention because of their improved physical properties compared to pure polymers or conventional microcomposites [1]. The addition of a nanometer scale filler may significantly improve the selected properties of the related polymer, namely mechanical, thermal, and barrier properties. It also provides a flame retardant character of polymers [2].Poly(butylene terephthalate) (PBT) is the semicrystalline engineering thermoplastic with good mechanical properties, good mouldability (low melting temperatureTm equal to about 496 K), and a fast crystallization rate [3]. The repeating units of poly(butylene terephthalate) (PBT) have flexible segment built from four methylene groups as well as a hard segment of a terephthalate group [4]. PBT has two crystalline modifications, the α and β forms, which both crystallize in a triclinic unit cell [5] and differ in the conformation of the central tetramethylene group. The α form exists in a relaxed state, whereas the β form is observed only under special processing conditions that imply the application of stress to unoriented molecular chains [6, 7]. The transition between the α form and β form is reversible and takes place by stretching and through relaxation. Moreover, in poly(butylene terephthalate) different types of spherulites were formed upon crystallization from the melt, in the same crystalline structure (α), depending on the crystallization conditions [7, 8]. PBT is often used as a matrix in nanocomposites because of its excellent moulding processing. The combination of outstanding electronic, conducting, and magnetic properties of fullerene C60 with the good processability of PBT seems to be promising for making improved polymeric material with novel physical and chemical properties. Due to the tendency of fullerene C60 towards agglomeration, the fullerene derivates, decylamine-C60 (DA-C60) and tetracyanoethylene oxide-C60 (TCNEO-C60), were synthesized. Then, new nanocomposites were obtained by direct reaction of PBT with fullerene adduct.In this paper, the influence of different concentrations of fullerene derivates on thermal properties of nanocomposites was investigated by the DSC method and it was compared with that of the virgin PBT data. The comparative studies of morphology of surfaces of the virgin PBT and of nanocomposites were carried out using scanning electron microscopy (SEM).


## 2. Experimental

### 2.1. Materials

Commercial grade PBT was supplied by Aldrich Company. The fullerene derivates,n-decylamine-C60 (DA-C60) and tetracyanoethylene oxide-C60 (TCNEO-C60), were prepared by the addition of n-decylamine and tetracyanoethylene oxide to fullerene C60 (Aldrich), respectively.To obtainn-decylamine-fullerene (DA-C60), 154 mg (0,214 mmol) fullerene C60 with 119 mg (0,642 mmol) n-decylamine was stirred at 303 K for 20 hours under argon. The crude product was precipitated by addition of 20 mL methanol to the reaction mixture and filtered off. The product was purified by extraction with chloroform (3×30mL) to give, after evaporation of solvent, 229 mg (84%) of n-decylamine-fullerene. The elemental analysis has confirmed monosubstitution of n-decylamine to fullerene C60.Tetracyanoethylene oxide-C60 (TCNEO-C60) adduct was obtained in the reaction of 200 mg (0.278 mmol) fullerene C60 and 40 mg (0.278 mmol) tetracyanoethylene oxide in toluene (150 mL). The reaction mixture was refluxed for 15 hours under argon. After evaporation of solvent, the brown solid residue was dissolved in chloroform and passed through Cellit. The eluate was evaporated under reduced pressure to give the solid product, which was dried in the vacuum desiccator (0.05 mmHg) at 298 K for 24 hours. The yield was 124 mg (52%). The purity of tetracyanoethylene oxide—C60 (TCNEO-C60) adduct was confirmed by elemental analysis, FTIR, and MS spectra.Fullerenation of PBT by direct reaction between DA-C60 and TCNEO-C60 was carried out according to the Olah method, using AlC13 as a catalyst [9]. To prepare PBT/n-decylamine-fullerene (PBT/DA-C60, 0,2% wt. of fullerene adduct), 5.0 g PBT was dissolved in 43,3 g 1,1,1,3,3,3-hexafluor-2-propanol and then 129,9 g chloroform, 50,0 mg anhydrous aluminum chloride, and 10,0 mg n-decylamine-fullerene (DA-C60) were added. The reaction mixture was refluxed for 10 hours under argon. The product was precipitated by addition of 500 g cold water to the chilled reaction mixture. The PBT/DA-C60 0,2% wt. of fullerene adduct (500 : 1) was filtered off and dried in the vacuum desiccator (0.05 mmHg) at 298 K for 24 hours. The PBT/TCNEO-C60 0,2% wt. of fullerene adduct was obtained in the same way using TCNEO-C60 instead of DA-C60. The other samples of PBT with fullerene adducts with different proportions, that is, 1000 : 1 (0.1% wt. of fullerene adduct) and 10000 : 1 (0.01% wt. of fullerene adduct), were prepared similarly, using 5.0 and 0.5 mg fullerene derivatives, respectively.


### 2.2. Differential Scanning Calorimetry (DSC)

The crystallization and melting studies of the virgin PBT and of the nanocomposites with different contents of fullerene derivates were carried out on a differential scanning calorimeter DSC Q2000 TA Instruments. Aluminium sample pans were used with sample weights in the region of 5 to 10 mg. The thermal parameters were obtained from the DSC thermograms of the sample heated up to 550 K and cooled down to 223 K and then reheated and recooled to the same temperatures as during the first cycle. All operations were performed at a rate of 10 K/min in a nitrogen atmosphere, using an empty aluminium sample pan as the reference. The first heating eliminated the influence of thermal history. The melting parameters from the reheating scans represent morphologies of samples crystallized from the melt under identical cooling conditions. The heat of crystallization was determined from the cooling scans. Glass transition temperatures(Tg) were estimated at the midpoint of the specific heat steps, while melting temperatures (Tm) and crystallisation temperatures (Tc) were measured at the maxima of the thermogram peaks. The melting enthalpies ΔHm and the crystallization enthalpies ΔHc were obtained from the areas of melting peaks and crystallization peaks, respectively.


### 2.3. SEM Study

The morphology of the PBT and nanocomposites was examined by scanning electron microscopy (SEM) using a Zeiss EVO-25 LS Scanning Electron Microscope operating with an acceleration voltage of 20 kV. The powder samples of PBT and the nanocomposites were dusted on the double-side conductive carbon films and then were coated with a thin gold layer in the order of nm by Balzers sputter coater SCD 050 in the atmosphere of argon.


## 2.1. Materials

Commercial grade PBT was supplied by Aldrich Company. The fullerene derivates,n-decylamine-C60 (DA-C60) and tetracyanoethylene oxide-C60 (TCNEO-C60), were prepared by the addition of n-decylamine and tetracyanoethylene oxide to fullerene C60 (Aldrich), respectively.To obtainn-decylamine-fullerene (DA-C60), 154 mg (0,214 mmol) fullerene C60 with 119 mg (0,642 mmol) n-decylamine was stirred at 303 K for 20 hours under argon. The crude product was precipitated by addition of 20 mL methanol to the reaction mixture and filtered off. The product was purified by extraction with chloroform (3×30mL) to give, after evaporation of solvent, 229 mg (84%) of n-decylamine-fullerene. The elemental analysis has confirmed monosubstitution of n-decylamine to fullerene C60.Tetracyanoethylene oxide-C60 (TCNEO-C60) adduct was obtained in the reaction of 200 mg (0.278 mmol) fullerene C60 and 40 mg (0.278 mmol) tetracyanoethylene oxide in toluene (150 mL). The reaction mixture was refluxed for 15 hours under argon. After evaporation of solvent, the brown solid residue was dissolved in chloroform and passed through Cellit. The eluate was evaporated under reduced pressure to give the solid product, which was dried in the vacuum desiccator (0.05 mmHg) at 298 K for 24 hours. The yield was 124 mg (52%). The purity of tetracyanoethylene oxide—C60 (TCNEO-C60) adduct was confirmed by elemental analysis, FTIR, and MS spectra.Fullerenation of PBT by direct reaction between DA-C60 and TCNEO-C60 was carried out according to the Olah method, using AlC13 as a catalyst [9]. To prepare PBT/n-decylamine-fullerene (PBT/DA-C60, 0,2% wt. of fullerene adduct), 5.0 g PBT was dissolved in 43,3 g 1,1,1,3,3,3-hexafluor-2-propanol and then 129,9 g chloroform, 50,0 mg anhydrous aluminum chloride, and 10,0 mg n-decylamine-fullerene (DA-C60) were added. The reaction mixture was refluxed for 10 hours under argon. The product was precipitated by addition of 500 g cold water to the chilled reaction mixture. The PBT/DA-C60 0,2% wt. of fullerene adduct (500 : 1) was filtered off and dried in the vacuum desiccator (0.05 mmHg) at 298 K for 24 hours. The PBT/TCNEO-C60 0,2% wt. of fullerene adduct was obtained in the same way using TCNEO-C60 instead of DA-C60. The other samples of PBT with fullerene adducts with different proportions, that is, 1000 : 1 (0.1% wt. of fullerene adduct) and 10000 : 1 (0.01% wt. of fullerene adduct), were prepared similarly, using 5.0 and 0.5 mg fullerene derivatives, respectively.


## 2.2. Differential Scanning Calorimetry (DSC)

The crystallization and melting studies of the virgin PBT and of the nanocomposites with different contents of fullerene derivates were carried out on a differential scanning calorimeter DSC Q2000 TA Instruments. Aluminium sample pans were used with sample weights in the region of 5 to 10 mg. The thermal parameters were obtained from the DSC thermograms of the sample heated up to 550 K and cooled down to 223 K and then reheated and recooled to the same temperatures as during the first cycle. All operations were performed at a rate of 10 K/min in a nitrogen atmosphere, using an empty aluminium sample pan as the reference. The first heating eliminated the influence of thermal history. The melting parameters from the reheating scans represent morphologies of samples crystallized from the melt under identical cooling conditions. The heat of crystallization was determined from the cooling scans. Glass transition temperatures(Tg) were estimated at the midpoint of the specific heat steps, while melting temperatures (Tm) and crystallisation temperatures (Tc) were measured at the maxima of the thermogram peaks. The melting enthalpies ΔHm and the crystallization enthalpies ΔHc were obtained from the areas of melting peaks and crystallization peaks, respectively.


## 2.3. SEM Study

The morphology of the PBT and nanocomposites was examined by scanning electron microscopy (SEM) using a Zeiss EVO-25 LS Scanning Electron Microscope operating with an acceleration voltage of 20 kV. The powder samples of PBT and the nanocomposites were dusted on the double-side conductive carbon films and then were coated with a thin gold layer in the order of nm by Balzers sputter coater SCD 050 in the atmosphere of argon.


## 3. DSC Results

### 3.1. Melting Behavior of the Virgin PBT and the Nanocomposites

Figure1 shows DSC heating curves of the virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites with different contents of DA-C60 and TCNEO-C60 fullerene derivates, respectively.Figure 1
The DSC first heating curves of the virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites with different contents of DA-C60 and TCNEO-C60 fullerene derivates, respectively.The melting parameters including the onset of melting(T1), melting peak temperatures (T2,T3), completion of melting (T4), the melting temperature range (T4-T1), the width of the melting peak, the melting enthalpy ΔHm and the degree of crystallinity (χc) were estimated from the first heating scans and collected in Table 1. All DSC curves show double overlapping melting peaks, which were explained based on the simultaneous melting and recrystallization of a distribution of crystallites of various sizes and different degrees of order [10].Table 1
DSC parameters obtained during the first heating for PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites, respectively.
Material with weight contents of fullerene derivateTg[K]Onset of meltingT1[K]Melting peak firstT2[K]Melting peak secondT3[K]Completion of meltingT4[K]Peak widthT4-T1[K]The melting enthalpyΔHm [J/g]The estimated value of the crystallinityχc [%]Virgin PBT328465485498508437251PBT/DA-C60 0.01% wt.331459489497506477553PBT/DA-C60 0.1% wt.335465495508437452PBT/DA-C60 0.2% wt.333457487498505487553PBT/TCNEO-C60 0.2% wt.333457488497504487553Controversy arises over the origin of the double melting behaviour of PBT. Initially, it was explained by the melting of crystals possessing differing morphologies or the melting of distributions of a single morphological form with a different size and perfection [11]. Then, the double melting behaviour of PBT was explained by the melt-recrystallization process [12, 13]. In this model the low-temperature endothermic peak was caused by the melting of original crystals formed during cooling, which have a low degree of perfection and wide distribution of crystals. The sharp high temperature peak was explained by the melting of reorganized more perfect crystals during a heating scan. It was attributed to a narrow distribution in thickness of lamellar crystallite.The degrees of crystallinity of the virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites were calculated according to the formula(1)χc=ΔHmΔHf100%,
as the ratio between the area of the endothermic peak (melting enthalpy ΔHm) and the theoretical value of enthalpy of homopolymer for 100% crystalline poly (butylene terephthalate) ΔHf=142 J/g [14, 15]. The estimated values of crystallinity χc presented in Table 1 slightly increase for nanocomposites in comparison with those for the virgin PBT.The melting range, which is the difference between the completion and the onset of melting(T4-T1), is wider in the nanocomposites as compared to that in the virgin PBT except for PBT/DA-C60 of 0.1% wt. of fullerene adduct, which is illustrated in Figure 2. These differences suggest that nanocomposites possess a wider distribution of crystal size than the virgin PBT. The temperature of the first melting peak was shifted towards higher temperatures for all nanocomposites, whereas the temperature of the second melting peak was insignificantly shifted to lower temperatures.Figure 2
The effect of the increasing of the peak width as a function of content fullerene derivates during the first heating for PBT/DA/C60 nanocomposites (circles) and for PBT/TCNEO/C60 nanocomposites (triangle).Figure3 presents the DSC reheating curves of virgin PBT, PBT/DA-C60, and of PBT/TCNEO-C60 nanocomposites with different contents of fullerene derivates, respectively. It was evident that DCS reheating thermograms of all samples show two distinct endothermic melting peaks. The small exothermic peaks between the double melting endothermic peaks in all DSC curves for PBT/TCNEO-C60 and for PBT/DA-C60 nanocomposites and for the virgin PBT confirm the hypothesis that melting of PBT proceeds through the process of melting of original crystals, recrystallization, and the melting of recrystallized crystals.Figure 3
The DSC second heating curves of virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites with different contents of fullerene derivates, respectively.The low-temperature peak was wide and has a small amplitude. It was connected with the melting of small crystallites, which have a wide size of distribution. The other melting peak in the higher temperature side was narrow and has a bigger amplitude. It means that large-size crystallites with narrower distribution melt in this temperature range [12]. Both the onset and the completion of melting for nanocomposites occurred in lower temperatures than those of the virgin PBT. The melting peak width (T4-T1) for nanocomposites presented in Figure 4 was bigger in comparison with that of the virgin PBT. It may indicate that, likewise during the first heating, the nanocomposites have less perfect crystallites with a broader distribution of crystallites size compared to those of the virgin PBT. The data on the melting behaviour for all the samples determined from the second heating are summarized in Table 3. The melting temperatures with the exception of the temperature of the melting of the first peak of PBT/DA-C60 of 0.2% wt. of fullerene adduct were kept about the same as those of the virgin PBT.Figure 4
The effect of increasing peak width as a function of content fullerene derivates during the second heating for PBT/DA-C60 nanocomposites (circles) and for PBT/TCNEO-C60 nanocomposites (triangle).The enthalpies of melting and recrystallization were calculated from the area under peaks. The degrees of crystallinity were estimated using the equation(2)χc=ΔHm1+ΔHm2-ΔHrecΔHf=ΔHmΔHf⋅100%,
where ΔHm1 is the melting enthalpy obtained from the first endothermic peak, ΔHm2 is the melting enthalpy obtained from the second endothermic peak, ΔHrec is the enthalpy of recrystallization, and ΔHf=142 J/g. The increase in the degree of crystallinity by 6% for PBT/DA-C60 of 0.01% wt. to 22% for PBT/DA-C60 of 0.1% of fullerene adduct in comparison with that for the virgin PBT could be explained on the basis of the heterogeneous nucleation provided by fullerene derivates in PBT [16].


### 3.2. Crystallization Behavior of the Virgin PBT and the Nanocomposites

Figures5 and 6 present the DSC thermograms of the virgin PBT and nanocomposites with different contents of DA-C60 and TCNEO-C60 adducts obtained during the first and the second cooling. The parameters characterizing the crystallization behavior obtained during the first and the second cooling such as the onset, completion, peak width, and enthalpy of the crystallization were collected in Tables 2 and 4, respectively.Table 2
DSC parameters obtained during the first cooling for PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites, respectively.
Material with weight contents of fullerene derivateOnset of crystallizationT5 [K]Peak crystallizationT6 [K]Completion of crystallizationT7 [K]Peak widthT7-T5 [K]Degree of supercoolingT3-T5 [K]The crystallization enthalpyΔHc [J/g]ΔHc/t [J/gs]Virgin PBT4754684611423600.71PBT/DA-C60 0.01% wt.4764694621421640.76PBT/DA-C60 0.1% wt.4784744641417640,76PBT/DA-C60 0.2% wt.4734644512225630,75PBT/TCNEO-C60 0.2% wt.4754684611422660,79Table 3
DSC parameters obtained during the second heating for PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites, respectively.
Material with weight contents of fullerene derivateOnset of meltingT1 [K]Melting peak firstT2 [K]Melting peak secondT3 [K]Completion of meltingT4 [K]Peak widthT4-T1 [K]The melting enthalpyΔHm [J/g]The estimated value of the crystallinityχc [%]Virgin PBT481485496501204632PBT/DA-C60 0.01% wt.478485495500224834PBT/DA-C60 0.1% wt.476486495499235539PBT/DA-C60 0.2% wt.476480495499235035PBT/TCNEO-C60 0.2% wt.475485495499245136Table 4
DSC parameters obtained during the second cooling for PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites, respectively.
Material with weight contents of fullerene derivateOnset of crystallizationT5 [K]Peak crystallizationT6 [K]Completion of crystallizationT7 [K]Peak widthT7-T5 [K]Degree of supercoolingT3-T5 [K]The crystallization enthalpyΔHc [J/g]ΔHc/t [J/gs]Virgin PBT4764684611520590,66PBT/DA-C60 0.01% wt.4774704641318640,82PBT/DA-C60 0.1% wt.4784744671117661PBT/DA-C60 0.2% wt.4734644522122620,5PBT/TCNEO-C60 0.2% wt.4774724661118630,95Figure 5
The DSC first cooling curves of virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites with different contents of fullerene derivates, respectively.Figure 6
The DSC second cooling curves of virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites with different contents of fullerene derivates, respectively.It was observed that the onset of crystallization(T5) of nanocomposites during the first and the second cooling was not altered significantly. The crystallization peak temperature (T6) measured at maximum crystallization rate, especially during the second cooling, indicates a tendency towards an increase. It was shifted towards higher temperatures by about a few degrees in comparison with that of the virgin PBT, which points to the modification of the nucleation process [17] and suggesting the accelerated crystallization of PBT fullerene nanocomposites. Only the PBT/DA-C60 sample of 0.2% wt. of fullerene adduct shows different behavior. Its characteristic crystallization temperatures were shifted to lower temperatures in comparison with those of the virgin PBT and other composites. Moreover, the peak of crystallization was very broad and has a lower amplitude. The crystallization behaviour of PBT/DA-C60 of 0.2% wt. of fullerene adduct is different from that of other studied samples, which may suggest that the process of crystallization is hindered for this nanocomposite. This sample will not be included in further considerations.In general, during the second cooling, nanocomposites exhibit a narrower width of exothermic crystallization peaks(T7-T5) by 2 K to 4 K than that of the virgin PBT with the exception of PBT/DA-C60 of 0.2% wt. of fullerene adduct. The heat of crystallization (ΔHc) increases for nanocomposites.The most important parameter describing the process of crystallization was the rate of crystallization. It is defined as the ratio of the heat of crystallization to the time, which is estimated between the onset and the completion of crystallization(ΔHc/t). The crystallization rate for nanocomposites was greater than that of the virgin PBT as given in Tables 2 and 4. The degree of supercooling (T3-T5) could be a measurement of a polymer crystallizability, what means that if the degree of supercooling is lower then the crystallization rate is greater [18]. The degrees of supercooling (T3-T5) collected in Tables 2 and 4 confirm that the overall crystallization rate for the nanocomposites is greater than that of the virgin PBT.The crystallization peak temperatures for all studied nanocomposites are higher than those of the virgin PBT; what is more is that nanocomposites are characterized by narrower crystallization peak width(T7-T5), smaller degree of supercooling (T3-T5), and greater crystallization rate (ΔHc/t). These results indicate that the crystallization is accelerated in nanocomposites.


### 3.3. The Glass Transition Temperature

Glass transition temperatures were estimated as the half-step temperature related to the change of heat capacity, which appears during the transition between the glassy and rubbery states. Figure7 collects the DSC thermograms of the studied samples in the vicinity of the glass transition temperature. The DSC results show increasing glass transition temperatures Tg for nanocomposites with increasing weight of the fullerene filler. The biggest increase in Tg by about 7 K was noticed for PBT/DA-C60 of 0.1% wt. of fullerene adduct. The observed increase of Tg may have been due to interfacial interaction in nanocomposites between the polymer matrix and the fullerene derivates [16, 17, 19, 20].Figure 7
The thermograms of the virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites with different contents of DA-C60 and TCNEO-C60 fullerene derivates in the vicinity of the glass transition temperature, respectively.


### 3.4. SEM Study

The surface analysis of SEM micrographs of the virgin PBT, PBT/DA-C60 0.01% wt., PBT/DA-C60 0.1% wt., PBT/DA-C60 0.2% wt., and PBT/TCNEO-C60 0.2% wt. nanocomposites presented in Figure 8 indicates a variation of surface morphology as a function of contents of fullerene derivates adduct. The increasing of the concentration of DA-C60 adduct from 0.01% wt. to 0.2% wt. leads to lower roughness of the surface of nanocomposites in comparison with that of the virgin PBT. The observed structure of the virgin PBT is fine-grained in comparison with that of nanocomposites. For nanocomposite PBT/TCNEO-C60 0.2% wt. a decrease in aggregates sizes was observed in comparison with those of PBT/DA-C60 nanocomposites, which could be explained by bigger chemical activity of TCNEO-C60 fullerene derivates.Figure 8
SEM micrographs of the virgin PBT, PBT/DA-C60 0.01%, PBT/DA-C60 0.1%, PBT/DA-C60 0.2%, and PBT/TCNEO-C60 0.2% nanocomposites, respectively.


## 3.1. Melting Behavior of the Virgin PBT and the Nanocomposites

Figure1 shows DSC heating curves of the virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites with different contents of DA-C60 and TCNEO-C60 fullerene derivates, respectively.Figure 1
The DSC first heating curves of the virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites with different contents of DA-C60 and TCNEO-C60 fullerene derivates, respectively.The melting parameters including the onset of melting(T1), melting peak temperatures (T2,T3), completion of melting (T4), the melting temperature range (T4-T1), the width of the melting peak, the melting enthalpy ΔHm and the degree of crystallinity (χc) were estimated from the first heating scans and collected in Table 1. All DSC curves show double overlapping melting peaks, which were explained based on the simultaneous melting and recrystallization of a distribution of crystallites of various sizes and different degrees of order [10].Table 1
DSC parameters obtained during the first heating for PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites, respectively.
Material with weight contents of fullerene derivateTg[K]Onset of meltingT1[K]Melting peak firstT2[K]Melting peak secondT3[K]Completion of meltingT4[K]Peak widthT4-T1[K]The melting enthalpyΔHm [J/g]The estimated value of the crystallinityχc [%]Virgin PBT328465485498508437251PBT/DA-C60 0.01% wt.331459489497506477553PBT/DA-C60 0.1% wt.335465495508437452PBT/DA-C60 0.2% wt.333457487498505487553PBT/TCNEO-C60 0.2% wt.333457488497504487553Controversy arises over the origin of the double melting behaviour of PBT. Initially, it was explained by the melting of crystals possessing differing morphologies or the melting of distributions of a single morphological form with a different size and perfection [11]. Then, the double melting behaviour of PBT was explained by the melt-recrystallization process [12, 13]. In this model the low-temperature endothermic peak was caused by the melting of original crystals formed during cooling, which have a low degree of perfection and wide distribution of crystals. The sharp high temperature peak was explained by the melting of reorganized more perfect crystals during a heating scan. It was attributed to a narrow distribution in thickness of lamellar crystallite.The degrees of crystallinity of the virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites were calculated according to the formula(1)χc=ΔHmΔHf100%,
as the ratio between the area of the endothermic peak (melting enthalpy ΔHm) and the theoretical value of enthalpy of homopolymer for 100% crystalline poly (butylene terephthalate) ΔHf=142 J/g [14, 15]. The estimated values of crystallinity χc presented in Table 1 slightly increase for nanocomposites in comparison with those for the virgin PBT.The melting range, which is the difference between the completion and the onset of melting(T4-T1), is wider in the nanocomposites as compared to that in the virgin PBT except for PBT/DA-C60 of 0.1% wt. of fullerene adduct, which is illustrated in Figure 2. These differences suggest that nanocomposites possess a wider distribution of crystal size than the virgin PBT. The temperature of the first melting peak was shifted towards higher temperatures for all nanocomposites, whereas the temperature of the second melting peak was insignificantly shifted to lower temperatures.Figure 2
The effect of the increasing of the peak width as a function of content fullerene derivates during the first heating for PBT/DA/C60 nanocomposites (circles) and for PBT/TCNEO/C60 nanocomposites (triangle).Figure3 presents the DSC reheating curves of virgin PBT, PBT/DA-C60, and of PBT/TCNEO-C60 nanocomposites with different contents of fullerene derivates, respectively. It was evident that DCS reheating thermograms of all samples show two distinct endothermic melting peaks. The small exothermic peaks between the double melting endothermic peaks in all DSC curves for PBT/TCNEO-C60 and for PBT/DA-C60 nanocomposites and for the virgin PBT confirm the hypothesis that melting of PBT proceeds through the process of melting of original crystals, recrystallization, and the melting of recrystallized crystals.Figure 3
The DSC second heating curves of virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites with different contents of fullerene derivates, respectively.The low-temperature peak was wide and has a small amplitude. It was connected with the melting of small crystallites, which have a wide size of distribution. The other melting peak in the higher temperature side was narrow and has a bigger amplitude. It means that large-size crystallites with narrower distribution melt in this temperature range [12]. Both the onset and the completion of melting for nanocomposites occurred in lower temperatures than those of the virgin PBT. The melting peak width (T4-T1) for nanocomposites presented in Figure 4 was bigger in comparison with that of the virgin PBT. It may indicate that, likewise during the first heating, the nanocomposites have less perfect crystallites with a broader distribution of crystallites size compared to those of the virgin PBT. The data on the melting behaviour for all the samples determined from the second heating are summarized in Table 3. The melting temperatures with the exception of the temperature of the melting of the first peak of PBT/DA-C60 of 0.2% wt. of fullerene adduct were kept about the same as those of the virgin PBT.Figure 4
The effect of increasing peak width as a function of content fullerene derivates during the second heating for PBT/DA-C60 nanocomposites (circles) and for PBT/TCNEO-C60 nanocomposites (triangle).The enthalpies of melting and recrystallization were calculated from the area under peaks. The degrees of crystallinity were estimated using the equation(2)χc=ΔHm1+ΔHm2-ΔHrecΔHf=ΔHmΔHf⋅100%,
where ΔHm1 is the melting enthalpy obtained from the first endothermic peak, ΔHm2 is the melting enthalpy obtained from the second endothermic peak, ΔHrec is the enthalpy of recrystallization, and ΔHf=142 J/g. The increase in the degree of crystallinity by 6% for PBT/DA-C60 of 0.01% wt. to 22% for PBT/DA-C60 of 0.1% of fullerene adduct in comparison with that for the virgin PBT could be explained on the basis of the heterogeneous nucleation provided by fullerene derivates in PBT [16].


## 3.2. Crystallization Behavior of the Virgin PBT and the Nanocomposites

Figures5 and 6 present the DSC thermograms of the virgin PBT and nanocomposites with different contents of DA-C60 and TCNEO-C60 adducts obtained during the first and the second cooling. The parameters characterizing the crystallization behavior obtained during the first and the second cooling such as the onset, completion, peak width, and enthalpy of the crystallization were collected in Tables 2 and 4, respectively.Table 2
DSC parameters obtained during the first cooling for PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites, respectively.
Material with weight contents of fullerene derivateOnset of crystallizationT5 [K]Peak crystallizationT6 [K]Completion of crystallizationT7 [K]Peak widthT7-T5 [K]Degree of supercoolingT3-T5 [K]The crystallization enthalpyΔHc [J/g]ΔHc/t [J/gs]Virgin PBT4754684611423600.71PBT/DA-C60 0.01% wt.4764694621421640.76PBT/DA-C60 0.1% wt.4784744641417640,76PBT/DA-C60 0.2% wt.4734644512225630,75PBT/TCNEO-C60 0.2% wt.4754684611422660,79Table 3
DSC parameters obtained during the second heating for PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites, respectively.
Material with weight contents of fullerene derivateOnset of meltingT1 [K]Melting peak firstT2 [K]Melting peak secondT3 [K]Completion of meltingT4 [K]Peak widthT4-T1 [K]The melting enthalpyΔHm [J/g]The estimated value of the crystallinityχc [%]Virgin PBT481485496501204632PBT/DA-C60 0.01% wt.478485495500224834PBT/DA-C60 0.1% wt.476486495499235539PBT/DA-C60 0.2% wt.476480495499235035PBT/TCNEO-C60 0.2% wt.475485495499245136Table 4
DSC parameters obtained during the second cooling for PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites, respectively.
Material with weight contents of fullerene derivateOnset of crystallizationT5 [K]Peak crystallizationT6 [K]Completion of crystallizationT7 [K]Peak widthT7-T5 [K]Degree of supercoolingT3-T5 [K]The crystallization enthalpyΔHc [J/g]ΔHc/t [J/gs]Virgin PBT4764684611520590,66PBT/DA-C60 0.01% wt.4774704641318640,82PBT/DA-C60 0.1% wt.4784744671117661PBT/DA-C60 0.2% wt.4734644522122620,5PBT/TCNEO-C60 0.2% wt.4774724661118630,95Figure 5
The DSC first cooling curves of virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites with different contents of fullerene derivates, respectively.Figure 6
The DSC second cooling curves of virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites with different contents of fullerene derivates, respectively.It was observed that the onset of crystallization(T5) of nanocomposites during the first and the second cooling was not altered significantly. The crystallization peak temperature (T6) measured at maximum crystallization rate, especially during the second cooling, indicates a tendency towards an increase. It was shifted towards higher temperatures by about a few degrees in comparison with that of the virgin PBT, which points to the modification of the nucleation process [17] and suggesting the accelerated crystallization of PBT fullerene nanocomposites. Only the PBT/DA-C60 sample of 0.2% wt. of fullerene adduct shows different behavior. Its characteristic crystallization temperatures were shifted to lower temperatures in comparison with those of the virgin PBT and other composites. Moreover, the peak of crystallization was very broad and has a lower amplitude. The crystallization behaviour of PBT/DA-C60 of 0.2% wt. of fullerene adduct is different from that of other studied samples, which may suggest that the process of crystallization is hindered for this nanocomposite. This sample will not be included in further considerations.In general, during the second cooling, nanocomposites exhibit a narrower width of exothermic crystallization peaks(T7-T5) by 2 K to 4 K than that of the virgin PBT with the exception of PBT/DA-C60 of 0.2% wt. of fullerene adduct. The heat of crystallization (ΔHc) increases for nanocomposites.The most important parameter describing the process of crystallization was the rate of crystallization. It is defined as the ratio of the heat of crystallization to the time, which is estimated between the onset and the completion of crystallization(ΔHc/t). The crystallization rate for nanocomposites was greater than that of the virgin PBT as given in Tables 2 and 4. The degree of supercooling (T3-T5) could be a measurement of a polymer crystallizability, what means that if the degree of supercooling is lower then the crystallization rate is greater [18]. The degrees of supercooling (T3-T5) collected in Tables 2 and 4 confirm that the overall crystallization rate for the nanocomposites is greater than that of the virgin PBT.The crystallization peak temperatures for all studied nanocomposites are higher than those of the virgin PBT; what is more is that nanocomposites are characterized by narrower crystallization peak width(T7-T5), smaller degree of supercooling (T3-T5), and greater crystallization rate (ΔHc/t). These results indicate that the crystallization is accelerated in nanocomposites.


## 3.3. The Glass Transition Temperature

Glass transition temperatures were estimated as the half-step temperature related to the change of heat capacity, which appears during the transition between the glassy and rubbery states. Figure7 collects the DSC thermograms of the studied samples in the vicinity of the glass transition temperature. The DSC results show increasing glass transition temperatures Tg for nanocomposites with increasing weight of the fullerene filler. The biggest increase in Tg by about 7 K was noticed for PBT/DA-C60 of 0.1% wt. of fullerene adduct. The observed increase of Tg may have been due to interfacial interaction in nanocomposites between the polymer matrix and the fullerene derivates [16, 17, 19, 20].Figure 7
The thermograms of the virgin PBT, PBT/DA-C60, and PBT/TCNEO-C60 nanocomposites with different contents of DA-C60 and TCNEO-C60 fullerene derivates in the vicinity of the glass transition temperature, respectively.


## 3.4. SEM Study

The surface analysis of SEM micrographs of the virgin PBT, PBT/DA-C60 0.01% wt., PBT/DA-C60 0.1% wt., PBT/DA-C60 0.2% wt., and PBT/TCNEO-C60 0.2% wt. nanocomposites presented in Figure 8 indicates a variation of surface morphology as a function of contents of fullerene derivates adduct. The increasing of the concentration of DA-C60 adduct from 0.01% wt. to 0.2% wt. leads to lower roughness of the surface of nanocomposites in comparison with that of the virgin PBT. The observed structure of the virgin PBT is fine-grained in comparison with that of nanocomposites. For nanocomposite PBT/TCNEO-C60 0.2% wt. a decrease in aggregates sizes was observed in comparison with those of PBT/DA-C60 nanocomposites, which could be explained by bigger chemical activity of TCNEO-C60 fullerene derivates.Figure 8
SEM micrographs of the virgin PBT, PBT/DA-C60 0.01%, PBT/DA-C60 0.1%, PBT/DA-C60 0.2%, and PBT/TCNEO-C60 0.2% nanocomposites, respectively.


## 4. Conclusion

The results confirm that the thermal properties as well as molecular dynamics [14, 21] of PBT/DA-C60 and PBT/TCNEO-C60 nanocomposites were changed in comparison with those of the virgin PBT. The studies of the melting and cooling processes show differences for the virgin PBT and PBT/DA-C60 and PBT/TCNEO-C60 nanocomposites. Fullerene derivates, DA-C60 and TCNEO-C60, affected the glass transition temperature, which indicates tendency towards shifting to higher temperatures.Analysis of DSC curves and SEM micrographs shows that nanocomposites possess crystallites with a broader distribution of size and a greater degree of crystallinity. It was shown that melting temperatures are not altered by fullerene derivates. The nanocomposites with the exception of PBT/DA-C60 of 0.2% wt. of fullerene adduct exhibit the narrower crystallization peak width, greater crystallization rate, and smaller degree of supercooling. These results suggest that fullerene derivates can act as heterogeneous nucleating agents in the nucleation of PBT crystallization, accelerating the process of crystallization.



---

*Source: 932573-2012-05-31.xml*